#------------------------------------------------------------------------------
#$Date: 2016-03-26 00:50:11 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180098 $
#$URL: svn://www.crystallography.net/cod/cif/7/05/44/7054460.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7054460
loop_
_publ_author_name
'Liu, Jia-min'
'Wang, Lu'
'Yu, Kai'
'Su, Zhan-hua'
'Wang, Chun-xiao'
'Wang, Chun-mei'
'Zhou, Bai-bin'
_publ_section_title
;
 Synthesis, crystal structure and properties of sandwich type compounds
 based on {AsW9} and a hexa-nuclear unit with three supporting
 TM--triazole complexes
;
_journal_issue                   2
_journal_name_full               'New J. Chem.'
_journal_page_first              1139
_journal_paper_doi               10.1039/C4NJ01138D
_journal_volume                  39
_journal_year                    2015
_chemical_formula_moiety         'C6 H26 As2 N9 Na9 Ni3 O73 W18'
_chemical_formula_sum            'C6 H26 As2 N9 Na9 Ni3 O73 W18'
_chemical_formula_weight         5234.22
_chemical_name_common            0012ljm
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           176
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   13.9035(10)
_cell_length_b                   13.9035(10)
_cell_length_c                   33.499(5)
_cell_measurement_reflns_used    7192
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.30
_cell_measurement_theta_min      2.43
_cell_volume                     5608.0(10)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1015
_diffrn_reflns_av_unetI/netI     0.0570
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       44
_diffrn_reflns_limit_l_min       -42
_diffrn_reflns_number            36180
_diffrn_reflns_theta_full        28.35
_diffrn_reflns_theta_max         28.35
_diffrn_reflns_theta_min         2.43
_exptl_absorpt_coefficient_mu    19.566
_exptl_absorpt_correction_T_max  0.0521
_exptl_absorpt_correction_T_min  0.0337
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
'Higashi, T. (1995). Program for Absorption Correction. Rigaku Corporation, Tokyo, Japan.'
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    3.100
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             4576.9
_exptl_crystal_size_max          0.36
_exptl_crystal_size_mid          0.34
_exptl_crystal_size_min          0.32
_platon_squeeze_details          ' ? '
_refine_diff_density_max         1.642
_refine_diff_density_min         -2.071
_refine_diff_density_rms         0.248
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.074
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     175
_refine_ls_number_reflns         4763
_refine_ls_number_restraints     48
_refine_ls_restrained_S_all      1.107
_refine_ls_R_factor_all          0.0759
_refine_ls_R_factor_gt           0.0574
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0654P)²+203.1337P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0928
_refine_ls_wR_factor_ref         0.1091
_reflns_number_gt                3699
_reflns_number_total             4763
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c4nj01138d2.cif
_cod_data_source_block           0012ljm
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Trigonal' changed to 'trigonal'
according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2827 2014-09-09 07:05:25Z andrius 

 Adding full bibliography for 7054460--7054462.cif.
;
_cod_original_cell_volume        5608.1(10)
_cod_database_code               7054460
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'x-y, x, z+1/2'
'-y, x-y, z'
'-x, -y, z+1/2'
'-x+y, -x, z'
'y, -x+y, z+1/2'
'-x, -y, -z'
'-x+y, -x, -z-1/2'
'y, -x+y, -z'
'x, y, -z-1/2'
'x-y, x, -z'
'-y, x-y, -z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_group
As1 As 0.3333 0.6667 0.16945(6) 0.0109(4) Uani 1 3 d SU .
W1 W 0.26378(5) 0.38703(4) 0.157423(16) 0.01449(15) Uani 1 1 d U .
W2 W 0.05505(5) 0.44502(5) 0.157450(16) 0.01474(15) Uani 1 1 d U .
W5 W 0.21202(5) 0.49238(5) 0.073841(16) 0.01939(16) Uani 1 1 d U .
Ni1 Ni 0.4096(2) 0.49859(19) 0.2500 0.0110(5) Uani 1 2 d S .
Na1 Na 0.1288(6) 0.3703(6) 0.2500 0.0109(4) Uani 1 2 d SU .
O1 O 0.2564(10) 0.2586(9) 0.1598(4) 0.030(3) Uani 1 1 d . .
O2 O 0.3707(8) 0.5838(8) 0.0682(3) 0.021(2) Uani 1 1 d U .
O3 O 0.2912(8) 0.4349(9) 0.2078(3) 0.0184(19) Uani 1 1 d U .
O4 O 0.1062(8) 0.3385(7) 0.1624(3) 0.017(2) Uani 1 1 d U .
O5 O 0.0912(9) 0.4891(9) 0.2082(3) 0.0189(18) Uani 1 1 d U .
O6 O 0.0709(8) 0.4301(8) 0.0979(3) 0.020(2) Uani 1 1 d U .
O7 O 0.2463(10) 0.5401(10) 0.1429(4) 0.0348(13) Uani 1 1 d U .
O8 O 0.2356(7) 0.3831(7) 0.0980(2) 0.0109(4) Uani 1 1 d . .
O9 O -0.0865(9) 0.3569(9) 0.1592(3) 0.027(2) Uani 1 1 d . .
O10 O 0.4180(10) 0.4789(10) 0.1432(4) 0.0348(13) Uani 1 1 d . .
O11 O 0.1734(11) 0.4378(11) 0.0262(3) 0.034(3) Uani 1 1 d . .
C1 C 0.4658(15) 0.3296(16) 0.2171(6) 0.037(4) Uani 1 1 d . .
H1A H 0.4621 0.3479 0.1907 0.045 Uiso 1 1 calc R .
N1 N 0.4520(13) 0.3798(14) 0.2500 0.018(3) Uani 1 2 d S .
N2 N 0.4860(18) 0.2478(16) 0.22978(15) 0.066(6) Uani 1 1 d D .
H2A H 0.4968 0.2040 0.2147 0.079 Uiso 0.50 1 calc PR .
O1W O 0.0000 0.0000 0.1079(11) 0.065(10) Uani 1 3 d S .
H1WA H -0.0156 0.0512 0.1044 0.077 Uiso 0.33 1 d PR .
H1WB H -0.0435 -0.0651 0.0992 0.077 Uiso 0.33 1 d PR .
O2W O 0.0000 0.0000 0.2150(13) 0.120(15) Uani 1 3 d S .
H2WA H -0.0070 0.0538 0.2235 0.144 Uiso 0.33 1 d PR .
H2WB H -0.0453 -0.0659 0.2225 0.144 Uiso 0.33 1 d PR .
O4W O 0.175(3) 0.198(3) 0.2500 0.035(5) Uani 0.50 2 d SPU .
H4WA H 0.1826 0.1720 0.2717 0.042 Uiso 0.50 1 d PR .
O5W O -0.026(3) 0.211(3) 0.2500 0.029(4) Uani 0.50 2 d SPU .
H5WA H -0.0714 0.1960 0.2690 0.034 Uiso 0.50 1 d PR .
H5WB H -0.0409 0.1654 0.2310 0.034 Uiso 0.50 1 d PR .
Na2 Na 0.1600(12) 0.0388(12) 0.1393(5) 0.0348(13) Uani 0.477(13) 1 d PU 2
Na2' Na 0.1428(11) 0.0332(11) 0.1716(4) 0.0348(13) Uani 0.523(13) 1 d PU 1
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ni Ni 0.3393 1.1124 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O7 As1 O7 97.6(5) 5_565 .
O7 As1 O7 97.6(5) 5_565 3_665
O7 As1 O7 97.6(5) . 3_665
O1 W1 O3 103.4(5) . .
O1 W1 O10 99.6(5) . .
O3 W1 O10 91.5(5) . .
O1 W1 O4 99.3(5) . .
O3 W1 O4 92.4(4) . .
O10 W1 O4 159.3(5) . .
O1 W1 O8 96.1(5) . .
O3 W1 O8 160.5(4) . .
O10 W1 O8 84.9(4) . .
O4 W1 O8 84.6(4) . .
O1 W1 O7 167.5(5) . .
O3 W1 O7 87.5(4) . .
O10 W1 O7 86.1(5) . .
O4 W1 O7 73.7(4) . .
O8 W1 O7 73.1(4) . .
O9 W2 O5 103.7(5) . .
O9 W2 O10 100.4(5) . 5_565
O5 W2 O10 91.7(5) . 5_565
O9 W2 O4 100.3(5) . .
O5 W2 O4 91.9(4) . .
O10 W2 O4 157.5(5) 5_565 .
O9 W2 O6 96.0(5) . .
O5 W2 O6 160.3(4) . .
O10 W2 O6 84.5(5) 5_565 .
O4 W2 O6 84.7(4) . .
O9 W2 O7 167.1(5) . .
O5 W2 O7 87.7(4) . .
O10 W2 O7 85.2(5) 5_565 .
O4 W2 O7 72.8(4) . .
O6 W2 O7 72.8(4) . .
O11 W5 O6 99.7(5) . .
O11 W5 O8 100.5(5) . .
O6 W5 O8 90.4(4) . .
O11 W5 O2 101.1(5) . 5_565
O6 W5 O2 89.3(4) . 5_565
O8 W5 O2 158.1(4) . 5_565
O11 W5 O2 101.6(5) . .
O6 W5 O2 158.5(4) . .
O8 W5 O2 88.3(4) . .
O2 W5 O2 84.1(6) 5_565 .
O11 W5 O7 171.4(5) . .
O6 W5 O7 74.4(4) . .
O8 W5 O7 73.6(4) . .
O2 W5 O7 85.3(4) 5_565 .
O2 W5 O7 84.7(4) . .
O5 Ni1 O5 89.0(6) 12_666 3_665
O5 Ni1 O3 159.8(4) 12_666 .
O5 Ni1 O3 87.2(4) 3_665 .
O5 Ni1 O3 87.2(4) 12_666 10_556
O5 Ni1 O3 159.8(4) 3_665 10_556
O3 Ni1 O3 89.5(6) . 10_556
O5 Ni1 N1 101.6(5) 12_666 .
O5 Ni1 N1 101.6(5) 3_665 .
O3 Ni1 N1 98.6(5) . .
O3 Ni1 N1 98.6(5) 10_556 .
O5 Ni1 Na1 45.0(3) 12_666 3_665
O5 Ni1 Na1 45.0(3) 3_665 3_665
O3 Ni1 Na1 125.2(3) . 3_665
O3 Ni1 Na1 125.2(3) 10_556 3_665
N1 Ni1 Na1 113.5(5) . 3_665
O5W Na1 O5 104.7(7) . 10_556
O5W Na1 O5 104.7(8) . .
O5 Na1 O5 70.9(5) 10_556 .
O5W Na1 O3 129.7(6) . 10_556
O5 Na1 O3 83.6(4) 10_556 10_556
O5 Na1 O3 124.4(5) . 10_556
O5W Na1 O3 129.7(6) . .
O5 Na1 O3 124.4(5) 10_556 .
O5 Na1 O3 83.6(4) . .
O3 Na1 O3 71.3(5) 10_556 .
O5W Na1 O4W 70.1(11) . .
O5 Na1 O4W 144.5(3) 10_556 .
O5 Na1 O4W 144.5(3) . .
O3 Na1 O4W 75.2(6) 10_556 .
O3 Na1 O4W 75.2(6) . .
O5W Na1 O4 82.6(2) . .
O5 Na1 O4 129.4(4) 10_556 .
O5 Na1 O4 59.0(3) . .
O3 Na1 O4 130.0(4) 10_556 .
O3 Na1 O4 59.1(3) . .
O4W Na1 O4 85.6(2) . .
O5W Na1 O4 82.6(2) . 10_556
O5 Na1 O4 59.0(3) 10_556 10_556
O5 Na1 O4 129.4(4) . 10_556
O3 Na1 O4 59.1(3) 10_556 10_556
O3 Na1 O4 130.0(4) . 10_556
O4W Na1 O4 85.6(2) . 10_556
O4 Na1 O4 164.7(5) . 10_556
O5W Na1 Ni1 113.3(9) . 8_566
O5 Na1 Ni1 35.8(3) 10_556 8_566
O5 Na1 Ni1 35.8(3) . 8_566
O3 Na1 Ni1 102.1(3) 10_556 8_566
O3 Na1 Ni1 102.1(3) . 8_566
O4W Na1 Ni1 176.6(8) . 8_566
O4 Na1 Ni1 94.7(2) . 8_566
O4 Na1 Ni1 94.7(2) 10_556 8_566
O5W Na1 W1 106.5(4) . 10_556
O5 Na1 W1 74.8(2) 10_556 10_556
O5 Na1 W1 138.2(3) . 10_556
O3 Na1 W1 26.9(2) 10_556 10_556
O3 Na1 W1 96.9(3) . 10_556
O4W Na1 W1 73.5(3) . 10_556
O4 Na1 W1 152.0(3) . 10_556
O4 Na1 W1 33.1(2) 10_556 10_556
Ni1 Na1 W1 105.09(13) 8_566 10_556
O5W Na1 W2 90.8(4) . 10_556
O5 Na1 W2 26.8(2) 10_556 10_556
O5 Na1 W2 96.4(3) . 10_556
O3 Na1 W2 74.7(2) 10_556 10_556
O3 Na1 W2 138.3(3) . 10_556
O4W Na1 W2 118.32(17) . 10_556
O4 Na1 W2 151.4(3) . 10_556
O4 Na1 W2 32.9(2) 10_556 10_556
Ni1 Na1 W2 62.33(10) 8_566 10_556
W1 Na1 W2 56.38(2) 10_556 10_556
O5W Na1 Na2' 43.9(4) . 3
O5 Na1 Na2' 139.7(4) 10_556 3
O5 Na1 Na2' 91.3(3) . 3
O3 Na1 Na2' 134.2(4) 10_556 3
O3 Na1 Na2' 87.3(3) . 3
O4W Na1 Na2' 60.0(5) . 3
O4 Na1 Na2' 42.7(3) . 3
O4 Na1 Na2' 122.0(3) 10_556 3
Ni1 Na1 Na2' 122.2(2) 8_566 3
W1 Na1 Na2' 130.5(3) 10_556 3
W2 Na1 Na2' 134.3(3) 10_556 3
W1 O1 Na2' 152.3(7) . .
W1 O1 Na2 151.4(7) . .
W5 O2 W5 153.0(6) 3_665 .
W1 O3 Ni1 143.7(6) . .
W1 O3 Na1 115.3(5) . .
Ni1 O3 Na1 99.2(4) . .
W2 O4 W1 120.3(5) . .
W2 O4 Na2 117.5(5) . 3
W1 O4 Na2 115.6(5) . 3
W2 O4 Na2' 124.5(5) . 3
W1 O4 Na2' 115.1(5) . 3
W2 O4 Na1 91.3(4) . .
W1 O4 Na1 91.0(4) . .
Na2 O4 Na1 113.9(5) 3 .
Na2' O4 Na1 91.3(4) 3 .
W2 O5 Ni1 143.7(6) . 8_566
W2 O5 Na1 115.8(5) . .
Ni1 O5 Na1 99.3(4) 8_566 .
W5 O6 W2 120.9(5) . .
As1 O7 W1 117.9(6) . .
As1 O7 W2 117.8(6) . .
W1 O7 W2 92.8(4) . .
As1 O7 W5 134.0(7) . .
W1 O7 W5 92.7(4) . .
W2 O7 W5 91.8(4) . .
W5 O8 W1 120.6(4) . .
W2 O10 W1 144.3(7) 3_665 .
N2 C1 N1 108.3(15) . .
N2 C1 H1A 125.9 . .
N1 C1 H1A 125.9 . .
C1 N1 C1 107(2) 10_556 .
C1 N1 Ni1 126.3(10) 10_556 .
C1 N1 Ni1 126.3(10) . .
N2 N2 C1 108.1(8) 10_556 .
N2 N2 H2A 125.9 10_556 .
C1 N2 H2A 125.9 . .
Na2 O1W Na2 100.2(11) 5 .
Na2 O1W Na2 100.2(11) 5 3
Na2 O1W Na2 100.2(11) . 3
Na2 O1W Na2' 86.3(11) 5 3
Na2 O1W Na2' 85.7(11) . 3
Na2 O1W Na2' 86.3(11) . 5
Na2 O1W Na2' 85.7(11) 3 5
Na2' O1W Na2' 67.9(9) 3 5
Na2 O1W Na2' 85.7(11) 5 .
Na2 O1W Na2' 86.3(11) 3 .
Na2' O1W Na2' 67.9(9) 3 .
Na2' O1W Na2' 67.9(9) 5 .
Na2 O1W H1WA 120.7 5 .
Na2 O1W H1WA 119.7 . .
Na2' O1W H1WA 57.8 3 .
Na2' O1W H1WA 115.1 5 .
Na2' O1W H1WA 115.2 . .
Na2 O1W H1WB 48.0 5 .
Na2 O1W H1WB 120.3 . .
Na2 O1W H1WB 130.0 3 .
Na2' O1W H1WB 128.3 3 .
Na2' O1W H1WB 70.2 5 .
Na2' O1W H1WB 120.5 . .
H1WA O1W H1WB 120.0 . .
Na2' O2W Na2' 84.7(13) 5 3
Na2' O2W Na2' 84.7(13) 5 .
Na2' O2W Na2' 84.7(13) 3 .
Na2' O2W H2WA 130.6 5 .
Na2' O2W H2WA 58.9 3 .
Na2' O2W H2WA 120.0 . .
Na2' O2W H2WB 56.4 5 .
Na2' O2W H2WB 127.7 3 .
Na2' O2W H2WB 120.0 . .
H2WA O2W H2WB 120.0 . .
Na1 O4W H4WA 120.3 . .
Na1 O5W Na2' 105.5(7) . 3
Na1 O5W Na2' 105.5(7) . 12_556
Na2' O5W Na2' 125.1(12) 3 12_556
Na1 O5W H5WA 119.2 . .
Na2' O5W H5WA 134.7 3 .
Na2' O5W H5WA 51.0 12_556 .
Na1 O5W H5WB 120.8 . .
Na2' O5W H5WB 111.8 12_556 .
H5WA O5W H5WB 120.0 . .
O1W Na2 O1 104.9(6) . .
O1W Na2 O4 128.7(6) . 5
O1 Na2 O4 125.9(6) . 5
O1W Na2 Na2 39.9(6) . 5
O1 Na2 Na2 127.9(6) . 5
O4 Na2 Na2 95.4(6) 5 5
O1W Na2 Na2 39.9(6) . 3
O1 Na2 Na2 70.1(6) . 3
O4 Na2 Na2 151.0(6) 5 3
Na2 Na2 Na2 59.999(1) 5 3
O2W Na2' O1 105.3(5) . .
O2W Na2' O4 124.4(7) . 5
O1 Na2' O4 125.1(6) . 5
O2W Na2' O1W 88.8(11) . .
O1 Na2' O1W 92.0(5) . .
O4 Na2' O1W 109.2(6) 5 .
O2W Na2' O5W 77.6(11) . 8_556
O1 Na2' O5W 99.0(8) . 8_556
O4 Na2' O5W 73.4(7) 5 8_556
O1W Na2' O5W 164.3(9) . 8_556
O2W Na2' Na2' 47.7(7) . 3
O1 Na2' Na2' 73.3(6) . 3
O4 Na2' Na2' 159.0(6) 5 3
O1W Na2' Na2' 56.1(5) . 3
O5W Na2' Na2' 116.6(6) 8_556 3
O2W Na2' Na2' 47.7(7) . 5
O1 Na2' Na2' 132.6(6) . 5
O4 Na2' Na2' 99.9(7) 5 5
O1W Na2' Na2' 56.1(5) . 5
O5W Na2' Na2' 108.4(7) 8_556 5
Na2' Na2' Na2' 60.000(1) 3 5
O2W Na2' Na1 88.7(8) . 8_556
O1 Na2' Na1 123.9(5) . 8_556
O4 Na2' Na1 45.9(3) 5 8_556
O1W Na2' Na1 143.3(4) . 8_556
O5W Na2' Na1 30.7(6) 8_556 8_556
Na2' Na2' Na1 136.0(3) 3 8_556
Na2' Na2' Na1 97.0(5) 5 8_556
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
As1 O7 1.796(12) 5_565
As1 O7 1.796(12) .
As1 O7 1.796(12) 3_665
W1 O1 1.738(11) .
W1 O3 1.785(10) .
W1 O10 1.928(13) .
W1 O4 1.950(10) .
W1 O8 2.026(8) .
W1 O7 2.311(13) .
W2 O9 1.722(11) .
W2 O5 1.793(10) .
W2 O10 1.925(12) 5_565
W2 O4 1.945(10) .
W2 O6 2.030(10) .
W2 O7 2.353(12) .
W5 O11 1.732(11) .
W5 O6 1.884(10) .
W5 O8 1.888(9) .
W5 O2 1.906(10) 5_565
W5 O2 1.927(10) .
W5 O7 2.388(12) .
Ni1 O5 1.996(10) 12_666
Ni1 O5 1.996(10) 3_665
Ni1 O3 2.008(10) .
Ni1 O3 2.008(10) 10_556
Ni1 N1 2.012(16) .
Ni1 Na1 3.371(8) 3_665
Na1 O5W 2.18(3) .
Na1 O5 2.414(11) 10_556
Na1 O5 2.414(11) .
Na1 O3 2.424(11) 10_556
Na1 O3 2.424(11) .
Na1 O4W 2.77(4) .
Na1 O4 2.960(10) .
Na1 O4 2.960(10) 10_556
Na1 Ni1 3.371(8) 8_566
Na1 W1 3.572(4) 10_556
Na1 W2 3.579(4) 10_556
O1 Na2' 2.742(17) .
O1 Na2 2.741(18) .
O2 W5 1.906(10) 3_665
O4 Na2 2.775(18) 3
O4 Na2' 2.795(17) 3
O5 Ni1 1.996(10) 8_566
O10 W2 1.925(12) 3_665
C1 N2 1.37(2) .
C1 N1 1.369(19) .
C1 H1A 0.9300 .
N1 C1 1.369(19) 10_556
N2 N2 1.354(10) 10_556
N2 H2A 0.8600 .
O1W Na2 2.27(2) 5
O1W Na2 2.27(2) .
O1W Na2 2.27(2) 3
O1W Na2' 2.79(3) 3
O1W Na2' 2.79(3) 5
O1W Na2' 2.79(3) .
O1W H1WA 0.8500 .
O1W H1WB 0.8500 .
O2W Na2' 2.31(3) 5
O2W Na2' 2.31(3) 3
O2W Na2' 2.31(3) .
O2W H2WA 0.8500 .
O2W H2WB 0.8500 .
O4W H4WA 0.8412 .
O5W Na2' 2.96(2) 3
O5W Na2' 2.96(2) 12_556
O5W H5WA 0.8500 .
O5W H5WB 0.8501 .
Na2 O4 2.776(17) 5
Na2 Na2 3.48(3) 5
Na2 Na2 3.48(3) 3
Na2' O4 2.795(17) 5
Na2' O5W 2.96(2) 8_556
Na2' Na2' 3.12(2) 3
Na2' Na2' 3.12(2) 5
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
N2 H2A O9 0.86 2.34 3.106(17) 148.7 5
O2W H2WA O4W 0.85 2.48 2.86(4) 108.3 .
O4W H4WA O1 0.84 2.56 3.187(17) 132.8 10_556
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O3 W1 O1 Na2' 87.5(15) . .
O10 W1 O1 Na2' -178.6(15) . .
O4 W1 O1 Na2' -7.2(16) . .
O8 W1 O1 Na2' -92.8(15) . .
O7 W1 O1 Na2' -62(3) . .
O3 W1 O1 Na2 137.8(14) . .
O10 W1 O1 Na2 -128.3(14) . .
O4 W1 O1 Na2 43.1(15) . .
O8 W1 O1 Na2 -42.4(15) . .
O7 W1 O1 Na2 -12(3) . .
O11 W5 O2 W5 129.5(13) . 3_665
O6 W5 O2 W5 -43(2) . 3_665
O8 W5 O2 W5 -130.2(13) . 3_665
O2 W5 O2 W5 29.3(15) 5_565 3_665
O7 W5 O2 W5 -56.5(13) . 3_665
O1 W1 O3 Ni1 74.7(10) . .
O10 W1 O3 Ni1 -25.5(10) . .
O4 W1 O3 Ni1 174.8(10) . .
O8 W1 O3 Ni1 -104.5(13) . .
O7 W1 O3 Ni1 -111.6(10) . .
O1 W1 O3 Na1 -85.3(6) . .
O10 W1 O3 Na1 174.5(6) . .
O4 W1 O3 Na1 14.8(5) . .
O8 W1 O3 Na1 95.4(12) . .
O7 W1 O3 Na1 88.4(6) . .
O5 Ni1 O3 W1 125.3(12) 12_666 .
O5 Ni1 O3 W1 45.8(10) 3_665 .
O3 Ni1 O3 W1 -154.2(7) 10_556 .
N1 Ni1 O3 W1 -55.5(10) . .
Na1 Ni1 O3 W1 71.4(11) 3_665 .
O5 Ni1 O3 Na1 -72.9(12) 12_666 .
O5 Ni1 O3 Na1 -152.5(5) 3_665 .
O3 Ni1 O3 Na1 7.6(6) 10_556 .
N1 Ni1 O3 Na1 106.2(5) . .
Na1 Ni1 O3 Na1 -126.8(3) 3_665 .
O5W Na1 O3 W1 35.0(11) . .
O5 Na1 O3 W1 -130.4(5) 10_556 .
O5 Na1 O3 W1 -68.8(6) . .
O3 Na1 O3 W1 161.5(3) 10_556 .
O4W Na1 O3 W1 82.5(7) . .
O4 Na1 O3 W1 -11.3(4) . .
O4 Na1 O3 W1 153.5(5) 10_556 .
Ni1 Na1 O3 W1 -99.6(5) 8_566 .
W1 Na1 O3 W1 153.3(4) 10_556 .
W2 Na1 O3 W1 -161.3(3) 10_556 .
Na2' Na1 O3 W1 22.8(5) 3 .
O5W Na1 O3 Ni1 -133.2(9) . .
O5 Na1 O3 Ni1 61.4(6) 10_556 .
O5 Na1 O3 Ni1 123.0(4) . .
O3 Na1 O3 Ni1 -6.6(5) 10_556 .
O4W Na1 O3 Ni1 -85.7(6) . .
O4 Na1 O3 Ni1 -179.5(5) . .
O4 Na1 O3 Ni1 -14.6(7) 10_556 .
Ni1 Na1 O3 Ni1 92.2(4) 8_566 .
W1 Na1 O3 Ni1 -14.9(4) 10_556 .
W2 Na1 O3 Ni1 30.5(7) 10_556 .
Na2' Na1 O3 Ni1 -145.4(4) 3 .
O9 W2 O4 W1 174.2(6) . .
O5 W2 O4 W1 -81.5(6) . .
O10 W2 O4 W1 17.6(15) 5_565 .
O6 W2 O4 W1 79.1(6) . .
O7 W2 O4 W1 5.5(5) . .
O9 W2 O4 Na2 24.0(7) . 3
O5 W2 O4 Na2 128.3(6) . 3
O10 W2 O4 Na2 -132.6(11) 5_565 3
O6 W2 O4 Na2 -71.1(6) . 3
O7 W2 O4 Na2 -144.7(7) . 3
O9 W2 O4 Na2' -1.4(7) . 3
O5 W2 O4 Na2' 102.9(6) . 3
O10 W2 O4 Na2' -158.0(11) 5_565 3
O6 W2 O4 Na2' -96.5(6) . 3
O7 W2 O4 Na2' -170.1(7) . 3
O9 W2 O4 Na1 -93.9(4) . .
O5 W2 O4 Na1 10.4(4) . .
O10 W2 O4 Na1 109.5(12) 5_565 .
O6 W2 O4 Na1 171.0(4) . .
O7 W2 O4 Na1 97.4(4) . .
O1 W1 O4 W2 -174.9(6) . .
O3 W1 O4 W2 81.2(6) . .
O10 W1 O4 W2 -19.5(16) . .
O8 W1 O4 W2 -79.5(6) . .
O7 W1 O4 W2 -5.6(5) . .
O1 W1 O4 Na2 -24.2(7) . 3
O3 W1 O4 Na2 -128.1(6) . 3
O10 W1 O4 Na2 131.3(12) . 3
O8 W1 O4 Na2 71.2(6) . 3
O7 W1 O4 Na2 145.2(7) . 3
O1 W1 O4 Na2' 1.1(7) . 3
O3 W1 O4 Na2' -102.8(6) . 3
O10 W1 O4 Na2' 156.5(12) . 3
O8 W1 O4 Na2' 96.5(5) . 3
O7 W1 O4 Na2' 170.4(6) . 3
O1 W1 O4 Na1 93.0(5) . .
O3 W1 O4 Na1 -10.9(4) . .
O10 W1 O4 Na1 -111.5(12) . .
O8 W1 O4 Na1 -171.6(4) . .
O7 W1 O4 Na1 -97.6(4) . .
O5W Na1 O4 W2 103.2(9) . .
O5 Na1 O4 W2 0.2(6) 10_556 .
O5 Na1 O4 W2 -9.0(4) . .
O3 Na1 O4 W2 -119.8(5) 10_556 .
O3 Na1 O4 W2 -111.0(4) . .
O4W Na1 O4 W2 173.6(8) . .
O4 Na1 O4 W2 118.3(17) 10_556 .
Ni1 Na1 O4 W2 -9.7(3) 8_566 .
W1 Na1 O4 W2 -145.3(5) 10_556 .
W2 Na1 O4 W2 25.1(8) 10_556 .
Na2' Na1 O4 W2 124.6(5) 3 .
O5W Na1 O4 W1 -136.5(9) . .
O5 Na1 O4 W1 120.5(5) 10_556 .
O5 Na1 O4 W1 111.4(4) . .
O3 Na1 O4 W1 0.5(6) 10_556 .
O3 Na1 O4 W1 9.3(3) . .
O4W Na1 O4 W1 -66.1(8) . .
O4 Na1 O4 W1 -121.4(17) 10_556 .
Ni1 Na1 O4 W1 110.6(3) 8_566 .
W1 Na1 O4 W1 -24.9(8) 10_556 .
W2 Na1 O4 W1 145.4(5) 10_556 .
Na2' Na1 O4 W1 -115.1(5) 3 .
O5W Na1 O4 Na2 -17.8(10) . 3
O5 Na1 O4 Na2 -120.8(6) 10_556 3
O5 Na1 O4 Na2 -130.0(6) . 3
O3 Na1 O4 Na2 119.2(6) 10_556 3
O3 Na1 O4 Na2 128.0(6) . 3
O4W Na1 O4 Na2 52.6(9) . 3
O4 Na1 O4 Na2 -3(2) 10_556 3
Ni1 Na1 O4 Na2 -130.8(5) 8_566 3
W1 Na1 O4 Na2 93.7(8) 10_556 3
W2 Na1 O4 Na2 -95.9(7) 10_556 3
Na2' Na1 O4 Na2 3.6(4) 3 3
O5W Na1 O4 Na2' -21.4(9) . 3
O5 Na1 O4 Na2' -124.4(6) 10_556 3
O5 Na1 O4 Na2' -133.6(5) . 3
O3 Na1 O4 Na2' 115.6(6) 10_556 3
O3 Na1 O4 Na2' 124.4(5) . 3
O4W Na1 O4 Na2' 49.0(8) . 3
O4 Na1 O4 Na2' -6(2) 10_556 3
Ni1 Na1 O4 Na2' -134.3(4) 8_566 3
W1 Na1 O4 Na2' 90.1(7) 10_556 3
W2 Na1 O4 Na2' -99.5(7) 10_556 3
O9 W2 O5 Ni1 -77.2(11) . 8_566
O10 W2 O5 Ni1 23.9(10) 5_565 8_566
O4 W2 O5 Ni1 -178.2(10) . 8_566
O6 W2 O5 Ni1 102.5(14) . 8_566
O7 W2 O5 Ni1 109.1(10) . 8_566
O9 W2 O5 Na1 86.9(6) . .
O10 W2 O5 Na1 -172.0(6) 5_565 .
O4 W2 O5 Na1 -14.2(6) . .
O6 W2 O5 Na1 -93.4(13) . .
O7 W2 O5 Na1 -86.9(6) . .
O5W Na1 O5 W2 -60.9(7) . .
O5 Na1 O5 W2 -161.7(3) 10_556 .
O3 Na1 O5 W2 130.6(5) 10_556 .
O3 Na1 O5 W2 68.5(6) . .
O4W Na1 O5 W2 15.3(16) . .
O4 Na1 O5 W2 10.8(4) . .
O4 Na1 O5 W2 -153.4(5) 10_556 .
Ni1 Na1 O5 W2 -170.5(8) 8_566 .
W1 Na1 O5 W2 161.7(3) 10_556 .
W2 Na1 O5 W2 -153.5(5) 10_556 .
Na2' Na1 O5 W2 -18.6(5) 3 .
O5W Na1 O5 Ni1 109.6(6) . 8_566
O5 Na1 O5 Ni1 8.8(5) 10_556 8_566
O3 Na1 O5 Ni1 -58.8(6) 10_556 8_566
O3 Na1 O5 Ni1 -121.0(4) . 8_566
O4W Na1 O5 Ni1 -174.2(13) . 8_566
O4 Na1 O5 Ni1 -178.7(5) . 8_566
O4 Na1 O5 Ni1 17.1(7) 10_556 8_566
W1 Na1 O5 Ni1 -27.8(7) 10_556 8_566
W2 Na1 O5 Ni1 17.0(4) 10_556 8_566
Na2' Na1 O5 Ni1 151.9(4) 3 8_566
O11 W5 O6 W2 172.3(6) . .
O8 W5 O6 W2 71.6(6) . .
O2 W5 O6 W2 -86.5(6) 5_565 .
O2 W5 O6 W2 -14.7(15) . .
O7 W5 O6 W2 -1.3(5) . .
O9 W2 O6 W5 -172.2(6) . .
O5 W2 O6 W5 8.1(16) . .
O10 W2 O6 W5 87.9(7) 5_565 .
O4 W2 O6 W5 -72.4(6) . .
O7 W2 O6 W5 1.3(5) . .
O7 As1 O7 W1 174.6(6) 5_565 .
O7 As1 O7 W1 75.8(10) 3_665 .
O7 As1 O7 W2 -75.4(10) 5_565 .
O7 As1 O7 W2 -174.1(6) 3_665 .
O7 As1 O7 W5 48.7(7) 5_565 .
O7 As1 O7 W5 -50.0(7) 3_665 .
O1 W1 O7 As1 -175(2) . .
O3 W1 O7 As1 34.5(7) . .
O10 W1 O7 As1 -57.2(7) . .
O4 W1 O7 As1 127.6(7) . .
O8 W1 O7 As1 -143.1(7) . .
O1 W1 O7 W2 61(2) . .
O3 W1 O7 W2 -89.2(4) . .
O10 W1 O7 W2 179.1(5) . .
O4 W1 O7 W2 4.0(4) . .
O8 W1 O7 W2 93.2(4) . .
O1 W1 O7 W5 -31(2) . .
O3 W1 O7 W5 178.8(5) . .
O10 W1 O7 W5 87.1(5) . .
O4 W1 O7 W5 -88.0(4) . .
O8 W1 O7 W5 1.2(3) . .
O9 W2 O7 As1 173.0(19) . .
O5 W2 O7 As1 -35.1(7) . .
O10 W2 O7 As1 56.8(7) 5_565 .
O4 W2 O7 As1 -127.8(8) . .
O6 W2 O7 As1 142.6(8) . .
O9 W2 O7 W1 -63(2) . .
O5 W2 O7 W1 88.7(5) . .
O10 W2 O7 W1 -179.4(5) 5_565 .
O4 W2 O7 W1 -4.0(4) . .
O6 W2 O7 W1 -93.6(5) . .
O9 W2 O7 W5 30(2) . .
O5 W2 O7 W5 -178.6(5) . .
O10 W2 O7 W5 -86.6(5) 5_565 .
O4 W2 O7 W5 88.8(4) . .
O6 W2 O7 W5 -0.9(4) . .
O6 W5 O7 As1 -131.9(10) . .
O8 W5 O7 As1 132.9(9) . .
O2 W5 O7 As1 -41.4(9) 5_565 .
O2 W5 O7 As1 43.2(9) . .
O6 W5 O7 W1 93.8(5) . .
O8 W5 O7 W1 -1.3(4) . .
O2 W5 O7 W1 -175.6(5) 5_565 .
O2 W5 O7 W1 -91.1(4) . .
O6 W5 O7 W2 0.9(4) . .
O8 W5 O7 W2 -94.2(4) . .
O2 W5 O7 W2 91.5(4) 5_565 .
O2 W5 O7 W2 176.0(5) . .
O11 W5 O8 W1 -171.8(6) . .
O6 W5 O8 W1 -71.9(6) . .
O2 W5 O8 W1 17.2(14) 5_565 .
O2 W5 O8 W1 86.7(5) . .
O7 W5 O8 W1 1.7(5) . .
O1 W1 O8 W5 171.6(6) . .
O3 W1 O8 W5 -9.2(15) . .
O10 W1 O8 W5 -89.3(6) . .
O4 W1 O8 W5 72.8(5) . .
O7 W1 O8 W5 -1.8(5) . .
O1 W1 O10 W2 -127.2(12) . 3_665
O3 W1 O10 W2 -23.4(12) . 3_665
O4 W1 O10 W2 77.4(18) . 3_665
O8 W1 O10 W2 137.4(12) . 3_665
O7 W1 O10 W2 64.0(12) . 3_665
N2 C1 N1 C1 1(3) . 10_556
N2 C1 N1 Ni1 -175.4(14) . .
O5 Ni1 N1 C1 46.4(17) 12_666 10_556
O5 Ni1 N1 C1 137.8(15) 3_665 10_556
O3 Ni1 N1 C1 -133.3(16) . 10_556
O3 Ni1 N1 C1 -42.5(16) 10_556 10_556
Na1 Ni1 N1 C1 92.1(16) 3_665 10_556
O5 Ni1 N1 C1 -137.8(15) 12_666 .
O5 Ni1 N1 C1 -46.4(17) 3_665 .
O3 Ni1 N1 C1 42.5(16) . .
O3 Ni1 N1 C1 133.3(16) 10_556 .
Na1 Ni1 N1 C1 -92.1(16) 3_665 .
N1 C1 N2 N2 -0.7(17) . 10_556
O5 Na1 O5W Na2' 149.8(8) 10_556 3
O5 Na1 O5W Na2' 76.1(10) . 3
O3 Na1 O5W Na2' -116.3(5) 10_556 3
O3 Na1 O5W Na2' -17.8(14) . 3
O4W Na1 O5W Na2' -67.1(8) . 3
O4 Na1 O5W Na2' 21.0(8) . 3
O4 Na1 O5W Na2' -155.1(10) 10_556 3
Ni1 Na1 O5W Na2' 112.9(8) 8_566 3
W1 Na1 O5W Na2' -132.0(6) 10_556 3
W2 Na1 O5W Na2' 173.0(8) 10_556 3
O5 Na1 O5W Na2' -76.1(10) 10_556 12_556
O5 Na1 O5W Na2' -149.8(8) . 12_556
O3 Na1 O5W Na2' 17.8(14) 10_556 12_556
O3 Na1 O5W Na2' 116.3(5) . 12_556
O4W Na1 O5W Na2' 67.1(8) . 12_556
O4 Na1 O5W Na2' 155.1(10) . 12_556
O4 Na1 O5W Na2' -20.9(8) 10_556 12_556
Ni1 Na1 O5W Na2' -112.9(8) 8_566 12_556
W1 Na1 O5W Na2' 2.1(11) 10_556 12_556
W2 Na1 O5W Na2' -52.9(9) 10_556 12_556
Na2' Na1 O5W Na2' 134.1(17) 3 12_556
Na2 O1W Na2 O1 -132.3(6) 5 .
Na2 O1W Na2 O1 -29.9(13) 3 .
Na2' O1W Na2 O1 -46.8(8) 3 .
Na2' O1W Na2 O1 -114.9(6) 5 .
Na2' O1W Na2 O1 -82.2(12) . .
Na2 O1W Na2 O4 39.7(18) 5 5
Na2 O1W Na2 O4 142.1(5) 3 5
Na2' O1W Na2 O4 125.2(9) 3 5
Na2' O1W Na2 O4 57.1(13) 5 5
Na2' O1W Na2 O4 89.9(15) . 5
Na2 O1W Na2 Na2 102.4(17) 3 5
Na2' O1W Na2 Na2 85.5(12) 3 5
Na2' O1W Na2 Na2 17.4(7) 5 5
Na2' O1W Na2 Na2 50.2(13) . 5
Na2 O1W Na2 Na2 -102.4(17) 5 3
Na2' O1W Na2 Na2 -16.9(6) 3 3
Na2' O1W Na2 Na2 -85.0(12) 5 3
Na2' O1W Na2 Na2 -52.2(13) . 3
W1 O1 Na2 O1W -10.0(19) . .
Na2' O1 Na2 O1W 104.4(15) . .
W1 O1 Na2 O4 177.7(12) . 5
Na2' O1 Na2 O4 -67.9(11) . 5
W1 O1 Na2 Na2 -46.9(17) . 5
Na2' O1 Na2 Na2 67.4(10) . 5
W1 O1 Na2 Na2 -29.9(13) . 3
Na2' O1 Na2 Na2 84.5(11) . 3
Na2' O2W Na2' O1 134.3(5) 5 .
Na2' O2W Na2' O1 49.2(10) 3 .
Na2' O2W Na2' O4 -70.0(14) 5 5
Na2' O2W Na2' O4 -155.1(6) 3 5
Na2' O2W Na2' O1W 42.6(6) 5 .
Na2' O2W Na2' O1W -42.6(5) 3 .
Na2' O2W Na2' O5W -129.6(9) 5 8_556
Na2' O2W Na2' O5W 145.2(10) 3 8_556
Na2' O2W Na2' Na2' 85.1(11) 5 3
Na2' O2W Na2' Na2' -85.1(11) 3 5
Na2' O2W Na2' Na1 -100.8(7) 5 8_556
Na2' O2W Na2' Na1 174.1(7) 3 8_556
W1 O1 Na2' O2W -28.2(19) . .
Na2 O1 Na2' O2W -138.9(16) . .
W1 O1 Na2' O4 176.3(12) . 5
Na2 O1 Na2' O4 65.6(11) . 5
W1 O1 Na2' O1W 61.1(16) . .
Na2 O1 Na2' O1W -49.6(11) . .
W1 O1 Na2' O5W -107.7(16) . 8_556
Na2 O1 Na2' O5W 141.6(14) . 8_556
W1 O1 Na2' Na2' 7.5(14) . 3
Na2 O1 Na2' Na2' -103.1(11) . 3
W1 O1 Na2' Na2' 17.6(18) . 5
Na2 O1 Na2' Na2' -93.0(11) . 5
W1 O1 Na2' Na1 -127.2(14) . 8_556
Na2 O1 Na2' Na1 122.2(13) . 8_556
Na2 O1W Na2' O2W -50.7(7) 5 .
Na2 O1W Na2' O2W 178.6(14) . .
Na2 O1W Na2' O2W 49.8(6) 3 .
Na2' O1W Na2' O2W 37.1(2) 3 .
Na2' O1W Na2' O2W -37.1(2) 5 .
Na2 O1W Na2' O1 -156.0(7) 5 .
Na2 O1W Na2' O1 73.3(12) . .
Na2 O1W Na2' O1 -55.5(7) 3 .
Na2' O1W Na2' O1 -68.2(7) 3 .
Na2' O1W Na2' O1 -142.4(5) 5 .
Na2 O1W Na2' O4 75.5(8) 5 5
Na2 O1W Na2' O4 -55.2(11) . 5
Na2 O1W Na2' O4 176.1(7) 3 5
Na2' O1W Na2' O4 163.3(6) 3 5
Na2' O1W Na2' O4 89.2(8) 5 5
Na2 O1W Na2' O5W -21(3) 5 8_556
Na2 O1W Na2' O5W -152(4) . 8_556
Na2 O1W Na2' O5W 79(3) 3 8_556
Na2' O1W Na2' O5W 66(3) 3 8_556
Na2' O1W Na2' O5W -8(3) 5 8_556
Na2 O1W Na2' Na2' -87.8(8) 5 3
Na2 O1W Na2' Na2' 141.5(14) . 3
Na2 O1W Na2' Na2' 12.8(6) 3 3
Na2' O1W Na2' Na2' -74.1(5) 5 3
Na2 O1W Na2' Na2' -13.6(6) 5 5
Na2 O1W Na2' Na2' -144.3(14) . 5
Na2 O1W Na2' Na2' 86.9(8) 3 5
Na2' O1W Na2' Na2' 74.1(5) 3 5
Na2 O1W Na2' Na1 35.5(14) 5 8_556
Na2 O1W Na2' Na1 -95.2(16) . 8_556
Na2 O1W Na2' Na1 136.0(8) 3 8_556
Na2' O1W Na2' Na1 123.3(8) 3 8_556
Na2' O1W Na2' Na1 49.1(12) 5 8_556
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
1 -0.016 -0.011 0.000 779.6 -1.0
2 -0.051 0.107 0.500 779.7 1.2
